ULTRA FIRE RESISTANTTHERMOSET POLYMERS Richard E. Lyon Fire Research Program Fire Safety Section AAR-440FEDERAL AVIATION ADMINISTRATION W.J. Hughes Technical Center Atlantic City International Airport, NJ 08405
ULTRA FIRE RESISTANT THERMOSET POLYMERS OUTLINE OF TALK • FAA Fire Resistant Materials Program • Background of Bisphenol-C Polymers • New Bisphenol-C Polymers • Fire & Flammability Results • Conclusions
A VERSATILE BUILDING BLOCK IS NEEDED Thermoplastics Thermosets
BACKGROUND: Bisphenol-C Polymers 1874: Chloral-phenol condensation reaction product (I) first reported. 1874: Dehydrochlorination to 1,1-dichloro, 2,2-bis(4-hydroxyphenyl) ethylene (bisphenol-C, BPC) first reported.
BACKGROUND: Bisphenol-C Polymers 1964: Polycarbonate from BPC first reported. 1965: “Self-Extinguishing Epoxies” from BPC first reported in Poland.
BACKGROUND: Bisphenol-C Polymers 1970’s: GE begins research to obtain non-burning (XB) plastics. Investigates bisphenol-C, etherimide, and acetylenic polymers. C.B. Quinn, 1967 • Acetylenic groups increase char yield in flame. • Too many acetylenes increase flammability (decrease LOI)
BACKGROUND: Bisphenol-C Polymers 1970’s: GE develops and patents industrial process chemistry to make BPC-polycarbonate (XB-1) and polyetherimide (XB-2). XB-1 XB-2 GE downselects to XB-2 (ULTEM™) because of fire (UL) and high temperature (TEM) capability.
BACKGROUND: Bisphenol-C Polymers 1980’s – 1990’s: Research in chloral condensation polymers continues in Poland and Russia but not in U.S.A. • Fire testing limited to flame tests (flammability). • High LOI (50-60) and “self-extinguishing” behavior attributed to chlorine content. • No commercial activity. 1994: Comprehensive review: Condensation Polymers Based on Chloral And Its Derivatives, A.L. Rusanov, Progress In Polymer Science, Vol. 19, pp. 589- 662 (1994)
BACKGROUND: Flaming Heat Release Rate Measured 1997: FAA measures flaming heat release rate of BPCpolycarbonate in OSU fire calorimeter.
BACKGROUND: New Flammability Screening Test 1998: FAA develops milligram-scale heat release rate test to accelerate search for new polymers Forced Nonflaming Combustion
HEAT RELEASE CAPACITY PREDICTS FIRE RESPONSE slope = 1 kg-K/m2-s (as per 1-D burning model) Provides new capability for rapid screening of research polymers for fire resistance.
BACKGROUND: Flammability Screening Yields Results 1998: FAA collaborates with Ciba Specialty Chemicals/Vantico Performance Polymers Division, Brewster, NY to develop ultra fire resistant cyanate ester thermoset resins for aircraft interiors BPC cyanate ester identified as having lowest heat release capacity of any thermoset tested to date BPC cyanate ester patent filed by Ciba/Vanitco BPC cyanate ester scaled-up and prepregged for bench scale fire calorimetry testing 1999-present: University (UMASS, Rice) research continues on BPC copolymers and blends.
BACKGROUND: Thermal Degradation Mechanism Identified 2000: “Thermal Decomposition Mechanism of…”, M. Ramirez, DOT/FAA/AR-00/42, and A. Factor, GE Plastics 350-450°C – 80 kJ/mole
BACKGROUND: Technology Transfer 2001: FAA Scales up BPC polycarbonate chemistry with Dow Chemical, Freeport TX 2002: U.S. Navy tests and approves BPC cyanate ester composites for use in submarines. 2003: VANTICO obtains composition of matter patent for BPC cyanate ester. 2004: NAVY awards SBIR programs to develop BPC thermoset process chemistry for large shipboard structures
BPC THERMOSET POLYMERS Epoxy Cyanate Ester Epoxy-Cyanate Ester Blends
EPOXY FORMULATIONS: Hardeners Examined EMI-24 (2 phr) TETA (14 phr) MDA (58 phr) BPC (78 phr DGEBC) BPA (66 phr DGEBA) Cyanate ester of BPC (53 phr DBEBC)
FIRE RESISTANCE OF BPC EPOXY LIMITED BY HIGH FUEL VALUE OF GLYCIDYL ETHER Dichloroethylidene (DCE) group has zero fuel value, but… “R” group for epoxy has relatively high fuel value. “R” Heat of combustion, hc = 7 kJ/g-polymer (theoretical) = 11 kJ/g-polymer (measured)
EPOXY HEAT RELEASE CAPACITIES DGEBA DGEBC UL 94 V-0 (typically)
EPOXY FIRE CALORIMETRY: Peak HRR Glass fabric lamina FAR 25.853 (a-1) DGEBA DGEBC FAA Maximum
EPOXY FIRE CALORIMETRY: Total Heat Release Glass fabric lamina FAR 25.853 (a-1) DGEBA DGEBC FAA Maximum (2-min, flaming)
MECHANICALS: BPA ( ) vs. BPC ( ) Epoxy STRENGTH STIFFNESS HEAT OF POLYMERIZATION GLASS TRANSITION TEMPERATURE
CYANATE ESTER: Polymerization Reaction BPC cyanate ester monomer 200°C BPC triazine thermoset polymer
EFFECT OF BISPHENOL ON HEAT RELEASE RATE OF CYANATE ESTERS ASTM 1354, cone calorimeter at 50 kW/m2 heat flux, neat resin, 1/4-inch thick
BPC CYANATE ESTER: FAA Heat Release Rate Test glass fabric lamina 1/8-in NOMEX honeycomb glass fabric lamina
STRUCTURAL COMPOSITES FOR NAVY SUBMARINES Only 3 resins pass fire performance requirements as glass composites: Fire Test/Characteristic Requirement (MIL-STD-2031) Composite Resin Phthalo- nitrile Silicone BPC-CE Time to ignition (s) at irradiance: 25 kW/m2 > 300 pass pass pass 50 kW/m2 > 150 pass pass pass pass pass pass 75 kW/m2 > 90 100 kW/m2 > 60 pass pass pass Peak/Average Heat Release Rate (kW/m2) at irradiance: 25 kW/m2 < 50/50 pass pass pass 50 kW/m2 < 65/50 pass pass pass pass pass pass 75 kW/m2 < 100/100 100 kW/m2 < 150/120 pass pass pass Smoke Obscuration, Dmax/Ds (avg): < 200/100 pass N/A pass Combustion Gas Toxicity (CO/CO2/HCN/HCl): pass N/A pass good good poor Mechanical Properties Cure Temperature < 200°C > 375°C N/A J. Koo, et. al., SAMPE 2001
CYANATE ESTER-EPOXY BLENDS
FIRE PERFORMANCE OF BPC(CE-EP) BLENDS 600 40 35 500 30 400 25 Heat Release Capacity of Blend, J/g-K 20 300 (Baseline Corrected) OSU Peak HRR, kW/m2 15 200 10 100 5 0 0 0 0.2 0.4 0.6 0.8 1 Mole Fraction BPC-Epoxy in Blend
CONCLUSIONS: Comparing Properties Average Change (5-7 polymers) BPC / BPA – 90 % Fire Hazard Potential (hc): Fire Hazard (HRR): – 60 % Glass Transition Temperature, K: + 3 % Modulus: + 10 % + 10 % Yield Strength: Yield Strain: + 10 %
ACKNOWLEDGEMENTS Jennifer Stewart, Huiquing Zhang, UMASS Lauren Castelli, Mike Ramirez, FAA Arnie Factor, Mike MacLaury, GE Plastics Borsheng Lin, Mike Amone, Ciba Specialty Chemicals Richard Walters, Galaxy Scientific Gary Green, Pacific Epoxy